O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a navegar o site, você aceita o uso de cookies. Leia nosso Contrato do Usuário e nossa Política de Privacidade.
O SlideShare utiliza cookies para otimizar a funcionalidade e o desempenho do site, assim como para apresentar publicidade mais relevante aos nossos usuários. Se você continuar a utilizar o site, você aceita o uso de cookies. Leia nossa Política de Privacidade e nosso Contrato do Usuário para obter mais detalhes.
The following presentation is only for quick reference. I would advise you to read the theoretical aspects of the respective topic and then use this presentation for your last minute revision. I hope it helps you..!!
Mayur D. Chauhan
Synthesis of Nanomaterials
Part II (Semester IV)
Paper I, Unit I
By: Mayur D. Chauhan
• Simple and Inexpensive, less instrumentation
compared to many physical methods
• Low temperature (<350oC) synthesis
• Doping of foreign atoms (Ions) is possible during
synthesis by either coupling, coating, chemical capping.
• Large quantities of the materials can be obtained with
a variety of sizes and shapes.
• Materials are obtained in the form of liquid but can be
easily converted into dry powder or thin films
• Self assembly or patterning is possible
• As in many cases nanoparticles synthesized by
chemical methods form what is known as
• A class of materials, in which two or more
phases (solid, liquid or gas) of same or
different materials co-exist with the
dimensions of at least one of the phases less
than a micrometre (μm) is known as colloids.
• Colloids may be particles, plates or fibres
• Nanomaterials are a subclass of colloids, in
which one of the dimensions is in nanometre
• Examples of Colloids: liquid in gas (fog), liquid
in liquid (fat droplets in milk), solid in liquid
(tooth paste), solid in solid (tinted glass), gas
in liquid (foam).
• Organic and inorganic materials can be
dispersed into each other to form colloids.
• Several examples exist even of bio-colloids.
Blood and bones are good examples of bio-
• Blood has corpuscles dispersed in serum and
bone has colloids of calcium phosphate
embedded in collagen.
• Colloids may even form networks. For
example aerogels are a network of silica
colloidal particles, pores of which are filled
Interactions of Colloids and Medium
• Colloids are particles with large surface to volume
• Correspondingly there are large number of
atoms/molecules on the surface of a colloidal
particle, which do not have as many neighbours
as those for an atom/molecule inside the interior.
• Therefore atoms on the surface are in a highly
reactive state, which easily interact to form
bigger particles or tend to coagulate.
• It is thus necessary to understand the stability
of colloids i.e. how the colloids dispersed in a
medium can remain as separated particles.
• We consider a case in which inorganic
spherical colloids of equal size are dispersed in
a liquid medium.
• When fine particles are dispersed in a liquid
medium, it is known that they undergo
• If we are able to tag a particle in the solution,
it would appear as if it is making a random
• All other particles also execute random
motion, hitting each other and changing
direction of motion in solution.
• Distance travelled between successive
collisions is random too.
Types of Interaction
Concept of Free Energy
• Free energy of a body is a measure of its ability to
• A body always tends to attain the state of lower
energy by releasing ‘free energy’
• In order to understand the meaning of surface
free energy, consider that a cylinder with cross
section ‘A’ and length ‘2l’ is cut into two equal
• Work has to be done in order to break the
cylinder into two pieces and separate them by a
• Energy increases as the distance between the
two pieces increases.
• The two pieces keep on attracting each other
due to intermolecular forces at the broken
interface. Therefore, more and more energy
has to be supplied in order to separate them.
• The force of attraction would increase in
vacuum but in a liquid medium the force of
attraction would reduce in general.
• With the help of this experiment, we
understand the interaction of colloidal
particles with the medium.
Effect of Charges on Colloids
• Colloids in liquid may be positively charged,
negatively charged or even neutral. But in
most of the cases they are charged.
• There are various sources for colloids by which
they acquire charges on their surfaces viz.
through composition of colloidal material,
properties of dispersing medium including the
type and concentration of dissolved ions in
• In any case as soon as there are some charges
on particles, ions of opposite charges
accumulate around them.
• Oppositely charged ions are known as Counter
ions. This accumulation of counter ions leads
to formation of an Electric double layer.
• Helmholtz considered that the situation is like
that in a parallel plate condenser, where there
are opposite charges separated through a
• Due to their Brownian motion, counter ions
are not fixed nor are colloidal particles at rest.
They execute their own Brownian motion and
form a dynamic double layer around them
• Consider now a situation in which two
charged colloidal particles come closer with
their electric double charge layers.
• As they approach each other, force of
repulsion increases. It is easy to see that the
difference in concentrations of double layer
charges would play an important role.
• Stability of colloids can be increased by
creating Stearic hindrance or repulsion.
• By adsorbing some layers of a different
material on colloidal particles e.g. polymer or
organic molecules on inorganic colloidal
particles, it is possible to reduce the attractive
forces between them.
• Addition of adsorbants would change the sizes
of the particles which helps them to stay at a
longer distance from each other, reducing the
• If the coating material is similar in properties
to that of the solvent, the effect of coating
would be negligible.
• Thus colloids interact with each other
dynamically and are affected by van der Waals
forces, colloid-colloid interaction mediated
through dispersing medium, electric double
layer and Stearic interactions.
• If the repulsive forces are strong enough,
colloids would be stabilized. Otherwise
ripening, coagulation, or network formation
may take place.
1. Synthesis of Colloids
• Synthesis of colloids is a very old method.
• Making nanoparticles using colloidal route
goes back to 19th century when M. Faraday
synthesized gold nanoparticles by wet
• The particles are so stable that even today the
colloidal solution made by him can be seen in
the British Museum in London.
• Chemical reactions in which colloidal particles
are obtained are carried out in some glass
reactor of suitable size.
• Glass reactor usually has a provision to
introduce some precursors, gases as well as
measure temperature and pH during the
reaction. It is usually possible to remove the
products at suitable time intervals.
• Reaction is usually carried out under inert
atmosphere like argon or nitrogen gas so as to
avoid any uncontrolled oxidation of the
• There is also a provision made to stir the
reactants during the reaction by using teflon-
coated magnetic needle.
• A = Homogenous Nucleation. Fast nucleation
takes place as the solute concentration
approaches a super saturation stage.
• B = Heterogeneous Nucleation. Aggregates
• C = Ostwald ripening process. Larger particles
tend to grow at the expense of smaller ones
thus becoming even larger.
• Heterogeneous nucleation lowers the energy
necessary for the nucleation of a particle.
• Consequently the critical size of the particles
is smaller in heterogeneous nucleation than
that for homogeneous nucleation.
2a. Synthesis of Metal Nanoparticles
by Colloidal Route
• Colloidal metal nanoparticles are often
synthesized by reduction of some metal salt or
• Example: Highly stable Gold particles can be
obtained by reducing Chloroauric acid
Stabilization by Electrochemical double
• Metal gold nanoparticles exhibit intense red,
magenta and other colors, depending upon
the particle size.
• Gold nanoparticles discussed above are
stabilized by repulsive Coulombic interactions.
• It is also possible to stabilize gold
nanoparticles using thiol or some other
• In a similar manner, silver, palladium, copper
and other metal nanoparticles can be
synthesized using appropriate precursors,
temperature, pH, duration of synthesis etc.
2b. Synthesis of Semiconductor
Nanoparticles by Colloidal Route
• Compound semiconductor nanoparticles can
be synthesized by wet chemical route using
• Sulphide semiconductors like CdS and ZnS can
be synthesized as nano-particles simply by
• To obtain ZnS nanoparticles any zinc salt like
zinc sulphate (ZnSO4), zinc chloride (ZnCl2),
zinc nitrate (ZnNO3) or zinc acetate
(Zn[CH3COO]2) can be dissolved in aqueous
medium and Na2S is added to the solution.
(One can even dissolve H2S gas in the Zn salt
• To obtain zinc oxide particles, we can use
• Once we get our desired nanoparticles, they
need to be surface passivated as colloids formed
in liquids have a tendency to coagulate or ripen
due to attractive forces existing between them.
• This is often known as ‘Chemical capping’.
• Advantage with this chemical route is that, one
can get stable particles of variety of materials not
only in the solution, but even after drying off the
• The coating, however, has to be stable and
noninteractive with the particle itself except at
• Chemical capping can be carried out at high or
low temperature depending on the reactants.
• In high temperature reactions, cold
organometallic reactants are injected in some
solvent like trioctylphosphineoxide (TOPO)
held at a temperature of 300–400 oC.
• For example when dimethyl cadmium [Cd(CH3)2]
and Se powder were injected in TOPO, CdSe
nanoparticles capped with PO4 groups were
• Although, this is a very good route of synthesizing
the nanoparticles, most of the organo-metallic
compounds are prohibitively expensive.
• Besides they are also toxic and difficult to handle.
Size Selective Precipitation
• In order to selectively obtain nanoparticles
with uniform sizes, one needs to use a proper
pair of solvent-nonsolvent liquids.
• Some of the solvent-nonsolvent pairs are
pyridine-hexane, chloroform-methanol or
dimethyl sulphoxide-diethyl ether.
• The nanoparticles are dispersed in a solvent so
as to get an optically clear solution.
• Nonsolvent solution is then added so that
• Supernatant and flocculate are separated by
• Precipitate has larger particles and can be
separated. Bigger particles, therefore, are first
separated from smaller particles and again
dispersed in the solvent solution.
• The process is continued until no change in
the size distribution is observed by repeating
Langmuir-Blodgett (LB) Method
• This technique to transfer organic overlayers
at air-liquid interface onto solid substrates is
known for nearly 70 years.
• The technique was developed by two
scientists Langmuir and Blodgett.
• In this technique, one uses amphiphilic long
chain molecules like that in fatty acids.
• For Example, consider the molecule of arachidic
acid, which has a chemical formula
• There are many such long organic chains with
• general chemical formula [CH3(CH2)nCOOH]where
n is a positive integer.
• In this case –CH3 is hydrophobic and –COOH is
hydrophilic in nature.
• Usually molecules with n>14 are candidates to
form L-B films
• When such molecules are put in water, the
molecules spread themselves on surface of
water in such a way that their hydrophilic
ends, often called as ‘heads’ are immersed in
water, whereas the hydrophobic ends called
as ‘tails’ remain in air.
• They are also surface active agents or
• Using a movable barrier, it is possible to compress
these molecules to come closer together to form
a ‘monolayer’ and align the tails.
• Such monolayers are two dimensionally ordered
and can be transferred on some suitable solid
substrates like glass, silicon etc.
• This is done simply by dipping the solid substrate
inside the liquid in which ordered organic
molecular monolayer is already formed.
• Depending upon the nature of substrate material
i.e. whether hydrophobic or hydrophilic, layers
are transferred on the solid substrates.
• A glass slide when dipped in the solution
becomes wet with water. Therefore, while it is
withdrawn from the liquid the head groups can
be easily attached to glass surface.
• As a result the whole monolayer gets transferred
in a manner as if a carpet is pulled.
• Now the glass substrate has tail groups, which
are hydrophobic on outer side.
• Therefore as it is dipped in the liquid again, it
acquires a second layer with tail – tail coming
closer together and while it is pulled back to
air, another monolayer of molecules with
head-head groups coming together is pulled.
• The process of dipping and pulling the
substrate can be repeated several times to
obtain ordered multilayers of molecules.
However to keep ordered layers available on
water surface, it is necessary to keep constant
pressure on the molecules.
• Whenever two immiscible liquids are
mechanically agitated or stirred together, they
are known to form an ‘emulsion’.
• The tendency of the liquids is such that the
liquid in smaller quantity tries to form small
droplets, coagulated droplets or layers so that
they are all separated from the rest of the
liquid in large quantity (for example droplets
of fat in milk).
• The droplet sizes in emulsions are usually
larger than 100 nm upto even few mm.
• Emulsions are usually turbid in appearance.
• On the other hand there is another class of
immiscible liquids, known as Microemulsions
which are transparent and the droplets are in
the range of 1–100 nm.
• Advantage of this method is the
biocompatibility and biodegradability of
• Biocompatibility is useful in novel applications
like drug delivery of nanomaterials and
biodegradability is useful to avoid
• Microemulsions are stabilized using
surfactants (surface stabilized active agents).
• When an organic liquid or oil (O), water (W)
and surfactant (T) are mixed together, under
some critical concentration, ‘micelles’ or
‘inverse micelles’ are formed, depending upon
the concentrations of water and organic
• The ratio of water (W), oil (O) and surfactant
(T) is important to decide which type of
micelle will be formed and can be represented
in a ternary phase diagram
• Composition can be determined by drawing
lines parallel to all three sides of the triangle
P = 60 % water, 26 % oil and 14 %
• A large number of nanoparticles (metals,
semiconductors and insulators) of cobalt,
copper, CaCO3, BaSO4, CdS or ZnS have been
synthesized using microemulsions or inverse
• Consider the synthesis of Co nanoparticles by
using sodium bis (2-ethylhexyl)sulfosuccinate
or Na(AOT)2 as a surfactant.
• A reverse micelle solution of water and oil can
be stabilized using a monolayer of surfactant
• The droplet diameter is controlled simply by
controlling the amount of water.
• Two micelle solutions having same diameter
of droplets can be formed.
• Thus one solution should have Co(AOT)2 i.e.
cobalt bis (2-ethylhexyl) sulfosuccinate and
the other should have sodium
tetrahydroborate (NaBH4 i.e. sodium
• When two solutions are mixed together the
resultant solution appears clear but the color
changes from pink to black.
• One can find by electron microscopy or some
other analysis that cobalt nanoparticles are
Sol – Gel Method
• Sol gels are known since the time when M.
Ebelman synthesized them in 1845.
• As the name suggests sol gel involves two
types of materials or components, ‘sol’ and
• Sols are solid particles in a liquid. They are
thus a subclass of colloids.
• Gels are nothing but a continuous network of
particles with pores filled with liquid (or
polymers containing liquid).
• A sol gel process involves formation of ‘sols’ in
a liquid and then connecting the sol particles
to form a network.
• By evaporating the liquid, it is possible to
obtain powders, thin films or even monolithic
• Sol gel method is particularly useful to
synthesize ceramics or metal oxides although
sulphides, borides and nitrides also are
• Sol gel formation is usually a low temperature
process. This means less energy consumption
and less pollution too.
• It competes with other processes like CVD or
metalloorganic vapours derived ceramics.
• It is also possible to synthesize nanoparticles,
nanorods or nanotubes using sol-gel
• Synthesis of sol-gel in general involves
hydrolysis of precursors, condensation
followed by polycondensation to form
particles, gelation and drying process.
• Precursors (starting chemicals) are to be
chosen so that they have a tendency to form
• Both Alkoxides or metal salts can be used.
• Alkoxides have a general formula M(ROH)n,
where M is a cation and R is an alcohol group, n is
the number of (ROH) groups with each cation.
• For example (ROH) can be methanol (CH3OH),
ethanol (C2H5OH), propanol (C3H7OH) etc.
bonded to a cation like Al or Si.
• Salts are denoted as MX, in which M is a cation
and X is an anion like in CdCl2, Cd is a cation and
Cl is an anion.
• By polycondensation process (i.e. many
hydrolyzed units coming together by removal
of some atoms from small molecules like OH),
sols are nucleated and ultimately sol-gel is
• Hydrothermal Synthesis
• Sonochemical Synthesis
• Microwave Synthesis
• Synthesis Using Micro-reactor or Lab-On-Chip